of guest-accessible amide functionalities. The amides are capable of base-catalyzing the Knoevenagel condensation of benzaldehyde with malononitrile. Reactions with larger nitriles, however, are only marginally accelerated, implying that catalysis takes place chiefly within the material's channels rather than on its exterior. A noteworthy finding is the lack of catalysis by the free strut in homogeneous solution, evidently due to intermolecular H-bonding between bptda molecules. Thus, the MOF architecture elicits catalytic activity not otherwise encountered. In an interesting alternative approach, Férey and coworkers were able to modify the interior of MIL-101 via Cr(III) coordination of one of the two available nitrogen atoms of each of several ethylenediamine molecules. The free non-coordinated ends of the ethylenediamines were then used as Brønsted basic catalysts, again for Knoevenagel condensation of benzaldehyde with nitriles. A third approach has been described by Kim Kimoon and coworkers. Using a pyridine-functionalized derivative of tartaric acid and a Zn(II) source they were able to synthesize a 2D MOF termed POST-1. POST-1 possesses 1D channels whose cross sections are defined by six trinuclear zinc clusters and six struts. While three of the six pyridines are coordinated by zinc ions, the remaining three are protonated and directed toward the channel interior. When neutralized, the noncoordinated pyridyl groups are found to catalyze transesterification reactions, presumably by facilitating deprotonation of the reactant alcohol. The absence of significant catalysis when large alcohols are employed strongly suggests that the catalysis occurs within the channels of the MOF. Achiral catalysis Metals as catalytic sites The metals in the MOF structure often act as Lewis acids. The metals in MOFs often coordinate to labile solvent molecules or counter ions which can be removed after activation of the framework. The Lewis acidic nature of such unsaturated metal centers can activate the coordinated organic substrates for subsequent organic transformations. The use of unsaturated metal centers was demonstrated in the cyanosilylation of aldehydes and imines by Fujita and coworkers in 2004. They reported MOF of composition {[Cd(4,4-bpy)2(H2O)2] • (NO3)2 • 4H2O} which was obtained by treating linear bridging ligand 4,4-bipyridine (bpy) with . The Cd(II) centers in this MOF possesses a distorted octahedral geometry having four pyridines in the equatorial positions, and two water molecules in the axial positions to form a two-dimensional infinite network. On activation, two water molecules were removed leaving the metal centers unsaturated and Lewis acidic. The Lewis acidic character of metal center was tested on